#------------------------------------------------------------------------------
#$Date: 2024-05-06 09:39:41 +0200 (Mon 06 de May de 2024) $
#$Revision: 291735 $
#$URL: svn://www.crystallography.net/cod/cif/9/00/97/9009730.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9009730
loop_
_publ_author_name
'Kusaka, K.'
'Ohmasa, M.'
'Hagiya, K.'
'Iishi, K.'
'Haga, N.'
_publ_section_title
;On variety of the Ca coordination in the incommensurate structure of
 synthetic iron-bearing akermanite, Ca2(Mg0.55,Fe0.45)Si2O7 Note: Sample is
 synthetic, this is the structure obtained from a standard refinement
;
_journal_name_full               'Mineralogical Journal'
_journal_page_first              47
_journal_page_last               58
_journal_paper_doi               10.2465/minerj.20.47
_journal_volume                  20
_journal_year                    1998
_chemical_formula_sum            'Ca2 Fe0.446 Mg0.554 O7 Si2'
_chemical_name_mineral           Akermanite
_space_group_IT_number           113
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.8679
_cell_length_b                   7.8679
_cell_length_c                   5.0144
_cell_formula_units_Z            2
_cell_volume                     310.411
_database_code_amcsd             0014431
_exptl_crystal_density_diffrn    3.067
_cod_original_formula_sum        'Ca2 (Mg.554 Fe.446) Si2 O7'
_cod_database_code               9009730
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
1/2-y,1/2-x,z
y,-x,-z
1/2-x,1/2+y,-z
-x,-y,z
1/2+y,1/2+x,z
-y,x,-z
1/2+x,1/2-y,-z
loop_
_atom_site_aniso_label
_atom_site_aniso_U_11
_atom_site_aniso_U_22
_atom_site_aniso_U_33
_atom_site_aniso_U_12
_atom_site_aniso_U_13
_atom_site_aniso_U_23
Ca 0.03073 0.03073 0.01121 0.02038 0.00160 -0.00160
Mg 0.01267 0.01267 0.01261 0.00000 0.00000 0.00000
Fe 0.01267 0.01267 0.01261 0.00000 0.00000 0.00000
Si 0.01239 0.01239 0.00853 0.00282 0.00190 -0.00190
O1 0.06335 0.06335 0.00637 0.05018 0.00000 0.00000
O2 0.03920 0.03920 0.00701 0.02509 0.00050 -0.00050
O3 0.07621 0.01819 0.01822 -0.01725 0.01799 -0.00500
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
Ca 0.33070 0.16930 0.50610 1.00000 0.02424
Mg 0.00000 0.00000 0.00000 0.55400 0.01267
Fe 0.00000 0.00000 0.00000 0.44600 0.01267
Si 0.13840 0.36160 0.93830 1.00000 0.01115
O1 0.00000 0.50000 0.82500 1.00000 0.04445
O2 0.13900 0.36100 0.25700 1.00000 0.02850
O3 0.07950 0.18980 0.78910 1.00000 0.03762
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0014431
